On the structure and oxygen transmission rate of biodegradable cellulose nanobarriers
© Chinga-Carrasco and Syverud; licensee Springer. 2012
Received: 9 September 2011
Accepted: 19 March 2012
Published: 19 March 2012
Cellulose nanofibrils have been proposed for novel barrier concepts, based on their capability to form smooth, strong and transparent films, with high oxygen barrier properties. A series of cellulose-based films were manufactured and tested with respect to their oxygen transmission rate (OTR) capabilities. The obtained OTR levels were considerably better than the levels recommended for packaging applications. Part of the nanofibrillated material applied in this study was produced with 2,2,6,6-tetramethylpiperidinyl-1-oxyl (TEMPO) mediated oxidation as pretreatment. Films made of TEMPO-pretreated samples yielded lower OTR values. The minimum obtained OTR value was 3.0 mL m-2 day-1 atm-1 with a corresponding oxygen permeability of 0.04 mL mm m-2 day-1 atm-1, tested at 50% relative humidity. The good barrier properties are due to the compact and dense structure of the films, as revealed by field-emission scanning electron microscopy. A relationship between OTR and the structure of the corresponding nanofibril-based films was confirmed.
KeywordsNanoparticles Polymers Porous materials Cellulose Films
Cellulose nanofibrils are nano-components of a cellulosic material produced through a fibrillation process . Several applications have been envisaged for cellulose nanofibrils due to their particular rheological, optical and strength properties [2–6]. The materials have also been proposed for packaging applications, based on their capability to form smooth, strong and transparent films, with high oxygen barrier properties [5, 7–10]. However, films made of cellulose nanofibrils are hydrophilic, having low moisture barrier properties. Surface modification has thus been proposed for reducing water wettability [7, 10, 11], which may be necessary in food packaging applications.
The density of nanofibril-based films is an important property to quantify, considering their potential application as barriers in packaging. The density gives an indication of the consolidation of the films during production. The more consolidated a given film is, the larger the density. Yang et al.  reported a relationship between the oxygen transmission rate (OTR) and the density of regenerated cellulose films. The intrinsic thickness of relatively thin films is an essential measure for estimating the density of the material. The thickness of cellulose films can be measured with electron microscopy techniques, as reported recently . In addition, the crystallinity degree of a given cellulose material has been reported to affect the OTR [5, 8], i.e. increasing the crystallinity degree reduces the oxygen permeability.
The purpose of this study is to shed light on the structure of nanofibril-based films and on how this complex structure limits the oxygen transmission rate through the material. A relationship between the structure of a series of nanofibril-based films and the corresponding OTR levels is confirmed.
A series of nanofibril qualities were utilized in this study. The nanofibril qualities were produced from Eucalyptus and Pinus radiata, as described by Syverud et al. . Some of the pulp fibres were chemically pretreated, according to Saito et al. . 2,2,6,6-Tetramethylpiperidinyl-1-oxyl (TEMPO) was applied to catalyse the oxidation of primary alcohol groups using NaClO. TEMPO-mediated oxidation facilitates a homogeneous fibrillation. A more detailed description is given by Syverud et al. .
Films were made from each series of the fibrillated materials
Homogenization (# passes)
Films (F01 to F08) were prepared in plastic petri dishes by free drying. The drying temperature was 23°C. Films of samples F01, F02 and F07 were additionally made in a cylindrical mould . The films made in the cylindrical mould are considered to be prepared in restrained conditions due to the supporting wire system. Film F07, made under restrained conditions, was additionally dried at 105°C for 2 h.
A scanning electron microscopy (SEM) cross-sectional analysis (thickness and roughness) was performed in backscatter electron imaging (BEI) mode as described by Chinga-Carrasco et al. . The applied microscope was a Hitachi S-3000 variable pressure SEM (Hitachi High-Technologies Corporation, Minato-ku, Tokyo, Japan), using a solid state backscatter detector. The densities of the films (δf) are given by the relationship γ/τf, where γ and τf correspond to the grammage and mean thickness of the films, respectively.
A surface structural quantification based on laser profilometry (LP; Lehmann, Lehman Mess-Systeme AG, Baden-Dättwil, Germany) and atomic force microscopy (AFM; Nanoscope Dimension 3100 controller, Digital Instruments-Vecco, Santa Barbara, CA, USA) was performed on the films, as described by Chinga-Carrasco et al.  and Syverud et al. . Ten local areas per sample were assessed with LP. The size of the local areas was 2 × 2 mm2, with a lateral resolution of 1 μm. The AFM analysis was performed on local areas of 5 × 5 μm2, with a lateral resolution of 10 nm.
The embedded films were exposed to a small quantity of water to induce a delamination of the cross-sectional structure. After drying, the samples were then covered with a conductive layer. Images were acquired at various magnifications with a field-emission SEM (Zeiss Ultra field-emission SEM, Carl Zeiss AG, Oberkochen, Germany). The images were acquired in secondary electron imaging (SEM-SEI) mode. In addition, a field-emission SEM analysis, applying the inlens detector, was performed for revealing the surface nanostructure of the films.
The OTR was measured with a Mocon OX-TRAN® 1/50 test system (Mocon, Minneapolis, MN, USA) at 50% relative humidity and 23°C.
Results and discussion
OTR values lower than 20 mL m-2 day-1 have been recommended for packaging applications . The OTR values of the films assessed in this study were between 3.0 and 4.4 mL m-2 day-1 atm-1. The lowest OTR level was 3.0 mL m-2 day-1 atm-1, which corresponds to an oxygen permeability of 0.04 mL mm m-2 day-1 atm-1. This is a good indication of the good barrier properties of the films, which are comparable to EVOH (3 to 5 mL m-2 day-1 atm-1)  and cellophane (3 mL m-2 day-1 atm-1) . For a comprehensive overview of the OTR levels of some renewable and synthetic polymers, see the study of Aulin et al. .
It is worth to notice that despite the major differences between the assessed films with respect to the nanofibril morphology and pore structure (Figure 1), the OTR values differ only by roughly 0.5 to 1.0 mL m-2 day-1 atm-1. This seems to confirm the poor connectivity of the pores in the film structures.
The Eucalyptus nanofibril-based films, made by free drying, yield lower densities than the corresponding P. radiata nanofibril-based films. One thus expected higher OTR values for the Eucalyptus nanofibril-based films. Eucalyptus films yield, however, similar OTR values at lower density (apparent higher porosity) compared to P. radiata (Figure 4, solid symbols). It was speculated whether the apparent lower density of the films, based on Eucalyptus nanofibrils, was caused by a relatively high shrinkage degree, as quantified by Syverud et al. . Shrinkage leads to higher mass per unit size. This thus leads to an underestimation of the quantified density, as the local grammage will be higher than the target grammage (20 g/m2). The density-OTR correlations should probably be translated to higher density levels, approaching the OTR-density correlation of the P. radiata nanofibril-based films. Films made under restrained conditions were analysed to verify this assumption. The OTR-density values of the films made under restrained conditions yielded variable results, probably due to the uneven structure caused by the formation procedure. However, the OTR-density measurements are in the same range as the measurements of the free-dried films and follow the same trend, i.e. increasing density reduces the OTR. This is a confirmation of the expected OTR-density relationship.
The obtained OTR levels of the films used in this study (grammage 20 g/m2) were considerably better than the levels recommended for packaging applications. Films made of TEMPO-pretreated samples yielded lower OTR values. The minimum obtained OTR was 3.0 mL m-2 day-1 atm-1 with a corresponding oxygen permeability of 0.04 mL mm m-2 day-1 atm-1, tested at 50% relative humidity. The good barrier properties are due to the compact and dense structure of the films. A relationship between OTR and the structure of the corresponding nanofibril-based films was confirmed.
atomic force microscopy
backscatter electron imaging
oxygen transmission rate
secondary electron imaging
scanning electron microscopy
transmission electron microscopy
The work was partly financed by the Research Council of Norway through the NanoFilter grant 196119/V30.
- Chinga-Carrasco G: Cellulose fibres, nanofibrils and microfibrils: the morphological sequence of MFC components from a plant physiology and fibre technology point of view. Nanoscale Rese Lett 2011, 6: 417. 10.1186/1556-276X-6-417View ArticleGoogle Scholar
- Turbak AF, Snyder FW, Sandberg KR: Microfibrillated cellulose, a new cellulose product: properties, uses, and commercial potential. J Appl Polym Sci Appl Polym Symp 1983, 37: 815–827.Google Scholar
- Taniguchi T, Okamura K: New films produced from microfibrillated natural fibres. Polymer Int 1998, 47: 291–294. 10.1002/(SICI)1097-0126(199811)47:3<291::AID-PI11>3.0.CO;2-1View ArticleGoogle Scholar
- Henriksson M, Berglund LA: Structure and properties of cellulose nanocomposite films containing melamine formaldehyde. J Applied Polymer Sci 2007, 106: 2817–2824. 10.1002/app.26946View ArticleGoogle Scholar
- Syverud K, Stenius P: Strength and permeability of MFC films. Cellulose 2009, 16(1):75–85. 10.1007/s10570-008-9244-2View ArticleGoogle Scholar
- Mörseburg K, Chinga-Carrasco G: Assessing the combined benefits of clay and nanofibrillated cellulose in layered TMP-based sheets. Cellulose 2009, 16(5):795–806. 10.1007/s10570-009-9290-4View ArticleGoogle Scholar
- Fukuzumi H, Saito T, Iwata T, Kumamoto Y, Isogai A: Transparent and high gas barrier films of cellulose nanofibers prepared by TEMPO-mediated oxidation. Biomac 2009, 10: 162–165. 10.1021/bm801065uView ArticleGoogle Scholar
- Aulin C, Gällstedt M, Lindström T: Oxygen and oil barrier properties of microfibrillated cellulose films and coatings. Cellulose 2010, 17: 559–574. 10.1007/s10570-009-9393-yView ArticleGoogle Scholar
- Siro I, Plackett D, Hedenqvist M, Ankerfors M, Lindström T: Highly transparent films from carboxymethylated microfibrillated cellulose: The effect of multiple homogenization steps on key properties. J Appl Polym Sci 2011, 119: 2652–2660. 10.1002/app.32831View ArticleGoogle Scholar
- Rodionova G, Lenes M, Eriksen Ø, Gregersen Ø: Surface chemical modification of microfibrillated cellulose: improvement of barrier properties for packaging applications. Cellulose 2010, 18(1):127–134.View ArticleGoogle Scholar
- Syverud K, Xhanari K, Chinga-Carrasco G, Yu Y, Stenius P: Films made of cellulose nanofibrils - surface modification by adsorption of a cationic surfactant and characterisation by computer-assisted electron microscopy. J Nanoparticle res 2010, 13(2):773–782.View ArticleGoogle Scholar
- Yang Q, Fukuzumi H, Saito T, Isogai A, Zhang L: Transparent cellulose films with high gas barrier properties fabricated from aqueous alkali/urea solutions. Biomac 2011, 12: 2766–2771. 10.1021/bm200766vView ArticleGoogle Scholar
- Chinga-Carrasco G, Yu Y, Diserud O: Quantitative electron microscopy of cellulose nanofibril structures from Eucalyptus and Pinus radiata kraft pulp fibres. Microsc Microanal 2011, 17: 563–571. 10.1017/S1431927611000444View ArticleGoogle Scholar
- Syverud K, Chinga-Carrasco G, Toledo J, Toledo P: A comparative study of Eucalyptus and Pinus radiata pulp fibres as raw materials for production of cellulose nanofibrils. Carbohyd Pol 2010, 84(3):1033–1038.View ArticleGoogle Scholar
- Saito T, Nishiyama Y, Putaux JL, Vignon M, Isogai A: Homogeneous suspensions of individualized microfibrils from TEMPO-catalyzed oxidation of native cellulose. Biomac 2006, 7(6):1687–1691. 10.1021/bm060154sView ArticleGoogle Scholar
- Henriksson M, Berglund LA, Isaksson P, Lindström T, Nishino T: Cellulose nanopaper structures of high toughness. Biomac 2008, 9(6):1579–1585. 10.1021/bm800038nView ArticleGoogle Scholar
- Parry RT: Principles and Applications of Modified Atmosphere Packaging of Foods. Suffolk: Chapman & Hall; 1993.View ArticleGoogle Scholar
- Kjellgren H, Engström G: Influence of base paper on the barrier properties of chitosan-coated paper. Nordic Pulp Paper Res J 2006, 21(5):685–689. 10.3183/NPPRJ-2006-21-05-p685-689View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.